View  Clemson University
J Mater Sci
DOI 10.1007/s108530104998y
Multilength scale modeling and analysis of microstructure
evolution and mechanical properties in polyurea
Mica Grujicic • B. Pandurangan • A. E. King •
J. Runt • J. Tarter • G. Dillon
Received: 8 July 2010 / Accepted: 8 October 2010
Ó Springer Science+Business Media, LLC 2010
Abstract A number of experimental investigations
reported in the open literature have indicated that polyurea
possesses a very complex nanometerscale material
microstructure consisting of hydrogenbonded discrete
hard (high glasstransition temperature, T g) domains and a
soft (low Tg) matrix and that the mechanical properties of
this type of elastomer are highly dependent on the details of
this microstructure. To help elucidate the internal processes/mechanisms
associated with the microstructure
evolution and to improve the understanding of microstructure/properties
in this material, a multilength scale
approach is developed and utilized in the present work.
This approach combines wellestablished and validated
atomic, meso, and continuum lengthscale techniques and
spans around six orders of magnitude of length (from
nanometers to millimeters). While within the atomicscale
approach, the material is modeled as a collection of constituent
atomsize particles, within the mesoscale approach
this atomistic description of the material is replaced with a
collection of coarser particles/beads which account for the
collective degrees of freedom of the constituent atoms. One
of the main efforts in the present work was the derivation
of accurate input parameters for mesoscale simulations
M. Grujicic (&) B. Pandurangan A. E. King
Department of Mechanical Engineering, Clemson University,
241 Engineering Innovation Building, Clemson, SC 296340921,
USA
email: mica.grujicic@ces.clemson.edu
J. Runt
Department of Material Science and Engineering, Pennsylvania
State University, University Park, PA 16082, USA
J. Tarter G. Dillon
Applied Research Laboratories, Pennsylvania State University,
University Park, PA 16082, USA
from the associated atomicscale material model and
results. The mesoscale analysis provided critical information
regarding the material microstructure and its evolution
(from an initially fully blended homogeneous state).
To obtain quantitative relationships between material
microstructure and its mechanical properties, the computed
mesoscale material microstructures are combined with a
finite element approach. The predictions of the present
multiscale computational approach are found to be in good
overall agreement with their experimental counterparts.
Introduction
Polyurea falls into a class of microphasesegregated and
thermoplastically crosslinked elastomeric copolymers
(the terms ‘‘microphasesegregated’’ and ‘‘thermoplastically
crosslinked’’ will be defined later) that are formed by
the rapid chemical reaction between isocyanates (organic
chemicals containing isocyanate –N=C=O groups) and
amines (organic chemicals containing amine –NH2
groups). A schematic of the polyurea copolymerization
reaction is shown in Fig. 1 in which symbol R is used to
represent an aromatic functional group (e.g., diphenyl
methane) while R 0 is used to denote an aromatic/aliphatic
long chain functional group (e.g., polytetramethyleneoxidediphenyl).
Since the copolymerization/gel reaction
times are typically less than a minute, polyurea synthesis
can be achieved under a wide range of temperatures and
humidity without significantly affecting material microstructure
and properties.
An examination of Fig. 1 reveals that the copolymerization
reaction creates urea linkages which are polar, i.e.,
contain centers/poles of negative and positive charge. Also
seen in Fig. 1 is that urea linkages together with the R
123
O=C=N N=C=O H2N NH2
R + R’
Where, R = CH2
and
O
R’ = C O C C C C O C
H H H H n
H
functional groups form the socalled ‘‘hard segments’’
(denoted as HS) within individual polyurea chains. Within
the same chains, R 0 functional groups form the socalled
‘‘soft segments’’ (denoted as SS). As a result of strong
hydrogen bonding between urea linkages of the neighboring
chains (or the neighboring portions of the same chain),
hard segments are typically microphase segregated into
the socalled ‘‘hard domains’’. An example of the formation
of hard domains within polyurea is shown schematically
in Fig. 2. As shown in this figure, nonphasesegregated
hard segments and soft segments form a soft
(i.e., low glass transition temperature, Tg) matrix. Since
hydrogen bonding provides interchain joining, polyureas
are often referred to as being thermoplastically crosslinked
(in contrast to more commonly covalently crosslinked)
polymers. Consequently, polyureas are described as segmented
(segmentcontaining) and thermoplastically crosslinked
(hydrogen bonding provides chain crosslinking)
elastomers. The hard domains typically possess a high
glass transition temperature (T g) and can crystallize under
suitable thermomechanical processing conditions [1].
Also, it should be noted that these domains act not only as
thermoplastic crosslinks but also as rigid reinforcements
within the continuous low Tg, compliant, and soft matrix.
H
H
Urealinkage, U

O O
H
RNCNR’NCN
H H H H n
Isocyanate Diamine Polyurea
Diphenyl Methane
Polytetramethyleneoxidediphenyl
Thus, Polyurea structure can be expressed as:
URUR’URUR’URUR’URUR’URUR’URU
Hard Segment, HS Soft Segment, SS
HSSSHSSSHSSSHSSSHSSSHSSS
Single Chain Molecular Structure
Fig. 1 Copolymerization reaction resulting in the formation of
segmented polyurea. To simplify the schematic of the molecular
structure, symbols HS (hard segment) and SS (soft segment) are used
123
O
HS SS HS SS HS
HS
SS
SS
HS
SS
HS
SSHS SS
HS
HS HS SS
SSHS
SS HS SS
SS
HS
SSHSSSHSSSHSSS
HS
SS
HS SS
SS
HS
SSHSSSHSSSHSSS
HS
HS
SS
SS
HS SSHS SS
SS
HS
HS
SS
SS
HS SSHS SS
HS
SS SSHS HS
HS SS
HS
SS SS HS
SS HS SS
Soft Matrix
Hard
Domain
Soft Matrix
J Mater Sci
Fig. 2 Schematic representation of the formation of hard domains
and the soft matrix within polyurea
Due to their highly complex internal microstructure
described above, polyureas display a very broad range of
mechanical responses under static and dynamic loading
conditions. The main features of these responses can be
defined as: (a) a highlevel of stress versus strain constitutive
nonlinearity; (b) extreme strainrate (and temperature)
sensitivity; and (c) a high degree of pressure
dependence. These types of mechanical responses have
favored the use of polyurea as an abrasion/corrosion protection
and blast/ballisticimpact mitigation material. For
instance, polyureas are frequently used as:
(a) Tough, abrasionresistant, corrosionresistant, durable,
and impactresistant (epoxy/rubber replacement)
sprayon coatings/liners in various construction/structural
applications such as tunnels, bridges, roofs,
parking decks, storage tanks, freight ships, truck beds,
etc.;
(b) External and internal wallsidings and foundation
coatings for buildings aimed at minimizing the degree
of structure fragmentation and, in turn, minimizing
the extent of the associated collateral damage in the
case of a bomb blast; and
(c) Gunfire/ballistic resistant and explosion/blast mitigating
coatings/liners or interlayers in blastresistant
sandwich panels for military vehicles and structures.
The applications mentioned above capitalize on the
exceptional ability of polyureas to harden under applied
loading and to alter/disperse shock waves and absorb the
kinetic energy associated with these waves/ballistic projectiles
(under dynamic loading conditions) [2, 3]. While it
is generally accepted that the high abrasion resistance and
the superior blast/ballisticimpact mitigation performance
of polyureas is the result of their intrinsic microstructure
[4], details regarding the relationships between the material
microstructure and the associated molecularlevel processes
and the macroscopic mechanical response of the
polyurea are not presently well understood.
J Mater Sci
In order to help gain insight into the molecularlevel
microstructure and processes and their effect on the macroscopic
mechanical response of polyurea, a multilength/
time scale procedure is introduced and employed in the
present work. To help understand the proposed multilength/time
scale procedure, a flow chart is depicted in
Fig. 3. It is seen that the procedure employs atomiclevel
methods, mesoscale level calculations and continuumlevel
finite element analysis. While ab initio quantum
mechanics methods have the advantage that they can, in
principle, be used for any element in the periodic table
without specific parameterization, they have a serious
shortcoming since they can be employed only for systems
containing no more than a few hundred atoms/particles. As
will be shown below, while ab initio quantum mechanics
calculations are not directly used in the present work, some
of the computational ab initio quantum mechanics results
are used in the parameterization of the material model at
the atomic length/time scale.
Fully atomistic computational methods, like the ones
used in the present work, in which each atom is uniquely
identified, rely on the application of molecular mechanics,
dynamics, and Monte Carlo algorithms to quantify the
response of polymeric materials. While most material
properties can be inferred from the application of these
methods, determination of the properties that are fundamentally
electronic (e.g., polarizability, dielectric constant,
rates of chemical reactions, etc.) typically entails the use
of either ab initio quantum mechanics or mesoscale
computational methods. The accuracy of properties
Fig. 3 A flow chart of the multilength/time scale computational
procedure proposed in the present work
predicted by the atomiclevel computational methods is
greatly dependent on accuracy and fidelity of the
employed force field (the mathematical expression used to
create the potential function of the interacting particles). In
the present work, the socalled ‘‘COMPASS’’ (Condensedphase
Optimized Molecular Potentials for Atomistic
Simulation Studies) force field is used [5, 6]. This highly
accurate force field is of an ab initio type since most of its
parameters were determined by matching the predictions
made by the ab initio quantum mechanics calculations to
the condensedmatter experimental data. In passing, it
should be recognized that the COMPASS force field is a
prime example of how the highly accurate results obtained
on one length/time scale (quantum mechanic/electronic, in
the present case) and the experimental data can be combined
to parameterize material models used at coarser
length/time scale (the atomistic length/time scale, in the
present case).
Within the fully atomistic methods described above,
materials response/properties are derived under the conditions
of constant material density, chemical composition,
and structure. Hence these methods are inherently suitable
only for pure (one component) or well mixed (multicomponent)
systems. When the system is multicomponental,
with limited component solubilities and the chain
topologies are highly complex, exotic phases are often
formed. Since these socalled ‘‘mesophases’’ comprise a
large number of items, their formation and properties
cannot be efficiently modeled using fully atomistic computational
methods. Instead, the socalled ‘‘coarsegrained’’
mesoscale computational methods become more suited in
these types of calculations. In these methods, longer length
scales are achieved by uniting many atoms into a single
entity called ‘‘bead’’ (each bead represents the collective
degrees of freedom of the constituent atoms) while longer
time scales are obtained by integrating out the high speed
movements of the constituent particles/atoms. This leaves
only the soft bead/bead interactions and low speed movements
of the beads. Hence, these methods are suitable for
studying more sluggish micronscale phase separation
phenomena such as the formation of hard domains and the
soft matrix in polyurea. It is critical to note that in order for
the mesoscale methods to yield reliable predictions, the
bead/bead interaction potentials must capture, in a meaningful
way, the underlying interactions of the constituent
atoms. Consequently, full atomicscale computational
methods are used to parameterize the mesoscale bead/bead
interaction potentials. This is another example of how the
highly accurate results obtained on one length/time scale
(the atomistic length/time scale, in the present case) and the
experimental data can be combined to parameterize material
models used at coarser length/time scale (meso length/
time scale, in the present case).
123
The main outcome of mesoscale computational analysis
is the prediction of the phase morphologies with characteristic
dimensions of the order of microns. While these
morphologies are of great interest, mesoscale computational
methods offer relatively little in terms of the prediction
of the associated physical and mechanical
properties of the material. To obtain these properties, one
can combine mesoscale predicted phasemorphology
results with a continuumlevel finite element computational
analysis. In this way, one can obtain a direct link between
the atomic and meso length/time scale material microstructure
and the macroscale material properties.
The organization of the paper is as follows: a brief
overview of the unit cell geometry and microstructure, the
computational method and the associated problem statement
for the atomicscale, mesoscale and continuumscale
analyses are presented in ‘‘Atomicscale calculations’’,
‘‘Mesoscale calculations’’, and ‘‘Continuumscale calculations’’
sections, respectively. The main results obtained
in the present work are presented and discussed in ‘‘Results
and discussion’’ section, while the key conclusions resulted
from the present study are summarized in ‘‘Summary and
conclusions’’ section.
(a)
H
C
Diphenyl Methane
Polyurea
Molecule
O
N
Linkage
Polytetramethyleneoxide
diphenyl
(b) (d)
Computational procedure
Atomicscale calculations
Formulation of an atomicscale simulation problem
requires, at a minimum, specification of the following three
aspects: (a) an atomicscale computational model consisting
of atoms, ions, functional groups, and/or molecules;
(b) a set of interaction potentials (commonly referred to as
force fields) which describe accurately various bonding and
nonbonding interaction forces between the constituents of
the atomicscale model; and (c) a computational method(s)
to be used in the simulation. More details of these three
aspects of the atomicscale modeling and simulations of
polyurea are provided below.
Computational model
The first step in the atomicscale computational analysis
was the construction of a single polyurea molecule. This
was carried out using the Visualizer [7] program from
Accelrys. A closeup view of a typical polyurea molecule
obtained is shown in Fig. 4a. For clarity, different atomic
(c)
H
C
O
Diphenyl Methane
N
Linkages
Hard Domain Molecule
J Mater Sci
Fig. 4 a A segment of a single polyurea molecule with the inset showing a zoomedout view of the same molecule; and b the atomicscale
computational unit cell in which, for clarity, each molecule is assigned a unique color
123
J Mater Sci
species and functional groups are labeled in this figure.
Also, a zoomedout view of a single polyurea molecule is
shown as an inset in Fig. 4a. It should be noted that the
polyurea molecule analyzed in the present work is based on
an isocyanate consisting of diphenyl methane (R) functional
group and a diamine consisting of polytetramethyleneoxidediphenyl
(R 0 ) functional group
(consisting of 14 C2H8O units), to comply with the type of
polyurea being investigated experimentally in our ongoing
work.
In order to model the behavior of bulk polyurea (i.e., in
the absence of any freesurface effects) at the atomic length
scale, a rectangular boxshaped computational unit cell is
constructed and the periodic boundary conditions are
applied across the faces of the cell. The three edges (a, b,
and c) of the cell are aligned, respectively, with the three
coordinate axes (x, y, and z). The atomic configuration
within the cell containing polyurea chains whose construction
was described in the previous section is generated
using the following procedure:
(a) The molecular chain constructed above is first grown
by a copyandattach process to increase its length/
molecular weight;
(b) The single polyurea chain constructed in (a) is next
used within the Amorphous Cell program from
Accelrys [8] to fill the rectangular boxshaped computational
cell of a preselected size (6.7 nm 9
6.7 nm 9 6.7 nm) while attaining the target density
(1300 kg/m 3 ) of polyurea; and
(c) The atomic configuration obtained in (b) is optimized
by minimizing its potential energy with respect to the
positions of the constituent atoms.
An example of the atomicscale computational cell used
in the present work is displayed in Fig. 4b. This cell contains
11,745 atoms of carbon, 18,900 atoms of hydrogen,
540 atoms of nitrogen, and 2,565 atoms of oxygen.
As discussed earlier, assynthesized polyurea is typically
microphase segregated and consists of hard domains and a
soft matrix. In contrast, the atomicscale polyurea model as
depicted in Fig. 4b represents a completely mixed state of
this material. As will be discussed later in detail, within the
atomicscale computational methods used, microphase
separation processes cannot be generally investigated.
Hence, atomicscale calculations based on the unit cell
displayed in Fig. 4b can only provide information about the
fully mixed material state/properties, i.e., information
about the material which resembles the softmatrix phase
of polyurea. It should be recalled that, within the softmatrix,
hard and soft segments are well mixed and, hence,
the atomicscale material model depicted in Fig. 4b isa
realistic representation of this phase of the polyurea. To
obtain atomicscale level information about the material
state/properties within the hard domains of polyurea, a new
moleculetype consisting of only hard segments and the
corresponding unit cell are used, Fig. 4c, d, respectively.
Force fields
While accurate simulations of a system of interacting
particles/atoms generally entail the application of quantum
mechanical techniques, such techniques are computationally
quite expensive and are usually feasible only in systems
containing up to a few hundreds of interacting
particles/atoms. In addition, the main goal of simulations of
systems containing a large number of particles/atoms is
generally to obtain the materials’ bulk properties which are
primarily controlled by the location of atomic nuclei.
Hence, the knowledge of the electronic structure, which is
the main outcome of the quantum mechanics computations,
is not critical. Under these circumstances, a good insight
into the behavior of a material system can be obtained if a
reasonable, physically based approximation of the potential
(force field) in which atomic nuclei move is available. Such
a force field can be used to generate a set of material
system configurations which are statistically consistent
with a fully quantum mechanical description of the same
system.
In the present molecularlevel analysis of polyurea,
COMPASS [5, 6] functional forms and parameterizations
were used for various bond and nonbond interaction
energies appearing in Eqs. 1–4. COMPASS is a set of force
field potentials which were derived through the use of
ab initio quantum mechanical calculations and has proven
to be highly accurate and reliable in starting various
organic/inorganic condensed matter problems. A schematic
explanation of the first four types of valence atomic
interactions included in the COMPASS force field is given
in Fig. 5. A summary of the COMPASS force field functions
can be found in our previous work [9].
b
( a)
φ
( b)
(c) (d)
Fig. 5 A schematic of the: a stretch, b angle, c torsion, and
d inversion valence atomic interactions
θ
χ
123
Computational method
Both molecular statics and molecular dynamics simulations
were employed in the present work. Within the molecular
statics approach, the unit cell potential energy (as defined
by Eqs. 1–4) is minimized with respect to the position of
the constituent particles/atoms. The potential energy minimization
within Discover [10] (the atomic simulation
program from Accelrys used in the present work) is carried
out by combining the Steepest Descent, Conjugate Gradient,
and the Newton’s minimization algorithms. These
algorithms are automatically inactivated/activated as the
atomic configuration is approaching its energy minimum
(i.e., the Steepest Descent method is activated at the
beginning of the energy minimization while the Newton’s
method is utilized in the final stages of the energy minimization
procedure).
Within the molecular dynamics approach, gradient of
the potential energy with respect to the particle positions is
first used to generate forces acting on the particles and,
then, the associated Newton’s equations of motion (for all
particles) are integrated numerically to track the temporal
evolution of the particle positions. More details regarding
the use of Discover to carry out molecular statics and
molecular dynamics analyses can be found in our prior
work [9].
Determination of the roomtemperature atomiclevel
mechanical properties of the two phases (soft matrix and
hard domains) within polyurea is accomplished by carrying
out the appropriate deformation of the computational cell
followed by combined application of molecular statics and
molecular dynamics analyses. These simulations yielded a
functional relationship between the internal energy and the
deformation state of the unit cell. As will be discussed in
detail in ‘‘Results and discussion’’ section, the mechanical
response of the two polyurea phases is obtained by
appropriate differentiation of this function. It should be
noted that while this procedure accounts for the contribution
of deformation to both the (bonding and nonbonding)
potential and vibrational energy components, changes in
the (configurational) entropy are not accounted for. To
assess the consequence of this simplification, the approach
described in Ref. [11] was considered. This approach
defines a dimensionless parameter and states that when this
parameter is significantly smaller than unity, entropy
effects can be neglected. Unfortunately, detailed temperature
and pressure dependencies of the material mechanical
response of polyurea needed to evaluate this parameter
were not available. Hence, the approach could not be
implemented.
The aforementioned deformations of the atomicscale
computational cell are carried out through the use of a
Discover input file [10] which is written in a Basic Tool
123
Command Language (BTCL) language. This enabled the
use of a scripting engine that provides very precise control
of simulation jobs, e.g., a cell deformation to be carried out
in small steps each followed by a combined energyminimization/moleculardynamics
simulation run. The energy
minimization procedure allows the system to reach the
condition of a minimum potential energy while the subsequent
molecular dynamics simulation enables the calculation
of the average potential and vibrational energies.
Typically, conventional NVT (N = 33,750, the number of
particles; V = 6.7 3 nm 3 , computational cell volume; and
T = 298 K, temperature; all kept constant) molecular
dynamics method was employed with 10,000 1.0 fs time
steps.
Problem formulation
As discussed earlier, atomicscale computational methods
used here are not suitable for the investigation of microphase
separation processes. The main reasons for this are as
follows:
(a) Within the molecular statics, local minimization
algorithms are employed which are capable of only
finding a minimum energy configuration of the given
(fully mixed or harddomain) state of the material;
and
(b) Molecular dynamics is dominated by high frequency
atomic vibrations and unrealizable computational
times are needed to simulate phase separation using
this approach.
Taking the above into consideration, atomicscale calculations
are employed in the present work for two main
purposes: (a) to generate the necessary parameters for use
in the mesoscale computational analysis; and (b) to
determine local mechanical properties of the soft matrix
and the hard domains within polyurea.
Mesoscale calculations
J Mater Sci
Within the mesoscale computational approach, the
atomicscale description of the molecules is coarsegrained
to form the socalled ‘‘beads’’ which represent the collective
degrees of freedom of all the constituent atoms. These
beads interact through pairpotentials which, in order to
obtain meaningful results, must capture the underlying
interactions between the constituent atoms. The procedures,
used to construct the appropriate mesoscale computational
unit cell and to derive bead–bead interaction
potentials from the corresponding atomicscale models and
results, are discussed in this section.
All the mesoscale calculations carried out in the present
work employed the socalled Mesodyn computational
J Mater Sci
method [12, 13]. At the mesoscale, the material system is
defined by prescribing bead properties (e.g., size/mass),
architecture of the polymer chains (e.g., chain length,
branching, etc.), and various bead mobility and interaction
parameters (e.g., bead selfdiffusion coefficients and the
interchain Flory–Huggins nonideal interaction parameters).
The temporal evolution of the system is governed by
a set of the socalled ‘‘functional Langevin equations’’ (one
for each beadtype) which are numerically solved. More
details regarding the Mesodyn computational method are
provided later in this section.
Computational cell
In order to model the behavior of a bulk material system,
an analogous approach was taken as in the case of atomicscale
calculations. That is, a rectangular boxshaped computational
cell (with an edge length which is approximately
an order of magnitude larger than its atomicscale counterpart)
was constructed and the periodic boundary conditions
applied to all of its faces. An example of the
conversion of the atomicscale material model into the
corresponding mesoscale material model is displayed in
Fig. 6a, b. In Fig. 6a, a segment of the mesoscale
molecular chain consisting of two bead types: A (red) and
B (blue), is displayed. The nature of the two beads will be
discussed later. In Fig. 6b, an example is provided of the
corresponding mesoscale unit cell used in the microstructureevolution
analysis of bulk polyurea.
The mesodyn computational method
As mentioned earlier, all the mesoscale calculations carried
out in the present work employed the socalled
Mesodyn computational method [12, 13]. Within this
method, polymer molecules are defined as ‘‘Gaussian
chains of beads’’. A Gaussian chain consists of orientationally
uncorrelated (freely jointed) links with the link
lengths (adjacent bead separation distances) following a
particular Gaussianrelated statistic. From the knowledge
of the expectation value for the link lengths, a distribution
of the endtoend chain lengths can be readily derived for
the Gaussian chains (using a randomwalk method). This,
in turn, leads to the determination of the corresponding
configurational entropy and for a given intrachain
Hamiltonian (an energy function which depends on the
distance of adjacent beads within the same chain) the
corresponding free energy.
Within the Mesodyn method, the temporal evolution of
the system is described by a set of socalled ‘‘functional
Langevin equations’’. Essentially, these equations represent
bead number density diffusion equations for different
components (bead types) in the material. However, in
(a)
(b)
Fig. 6 a A segment of the mesoscale model for a single Gaussianchain
of polyurea consisting of two types of beads A (red/light) and
B(blue/dark); and b the mesoscale computational unit cell used to
model bulk polyurea (Color figure online)
contrast to the common diffusion equations, these equations
each contain a random noise term (which enables the
system to escape a local freeenergy minimum associated
with a metastable state of the system). Within the Mesodyn
method, the driving force for bead number density evolution
is the existence of a nonzero gradient of the corresponding
intrinsic chemical potential. The later is obtained
by differentiating the free energy functional with respect to
the corresponding bead number density field. Temporal
evolution of the component’s density (from the initially
homogeneous mixture), is computed by numerically
inverting the Langevin equations.
The Mesodyn computational method is based on a
dynamic variant of meanfield density functional theory
which postulates that the free energy, F, of a heterogeneous
material system is a functional of the local bead number
density field, q and that there is a onetoone correspondence
between the bead spatialdistribution function in the
system, the material density field and an externally applied
potential field (a fieldtype lagrangianmultiplier function).
Since the free energy is a thermodynamic potential, all other
thermodynamic quantities can be derived from it through
proper differentiation and the associated thermodynamic
processes analyzed. For example, phase separation can be
123
detected by monitoring spatial distribution of the bead
number density within the system.
All the mesoscale computational analysis carried out in
the present work were done using Mesodyn computer
program from Accelrys [13].
Derivation of the mesoscale material model parameters
In this section, details regarding the derivation of the two
key mesoscale materialmodel parameters (i.e., bead’s
size/length along the chain and the Flory–Huggins interaction
parameter between beads) are presented.
Beadsize/length determination Before the bead lengths
could be determined, one must select the atomic makeup
of the beads and the number of bead types. As mentioned
earlier, in order to keep the mesoscale material model
relatively simple, the system is assumed to consist of two
bead types (A and B). Based on the polyurea chain
molecularlevel structure (e.g., Fig. 1), it was decided to
define two A beads as an assembly of one R functional
group surrounded by two urea linkages and then by two
phenyl groups (it should be noted that the latter are components
of the R 0 functional group, Fig. 1). Before the
molecularlevel structure of the bead B can be determined,
it had to be recognized, as will be shown below, that the
volumes of beads A and B have to be comparable. In order
to determine the volume of the bead A, a series of
molecular dynamics calculations were carried out using
polyurea chains with the number of repeat C 4H 8O units
within the R 0 functional group increasing between 14 and
30. Volumes of the bead A and the C4H8O repeat units are
then calculated from the resulting material specific volume
change under the assumption that this specific volume is a
linear combination of the (constant) specific volumes of
these two species. Using this procedure, it was determined
that the volume of three C4H8O repeat units (3 9
71.23 = 213.69 cm 3 /mol) is approximately equal to the
volume of one A bead (1 9 209.8 cm 3 /mol). Based on this
finding, mesoscale Gaussian chains were assigned the
following structure: A–A–B–B–B–B–B–A–A–B–B–B–B–
B…. The same procedure identified an average bead length
along the chain of 1.6 nm.
Determination of bead–bead interaction parameters
Bead/bead Flory–Huggins interaction parameters are
determined in the present work using the socalled Hildebrand’s
formula [14]. Within this formula, the Flory–
Huggins interaction parameter v AB is given by:
ð Þ 2
v AB ¼ dA dB
123
RT
Vref
ð1Þ
where V ref is the reference (i.e., the mean) volume of
interacting beads and dI (I = A, B) is the bead solubility
parameter. The latter is equal to the square root of the
corresponding bead volumetric cohesiveenergy density,
where the bead cohesive energy density is a measure of the
potential energy decrease, per unit volume, in a polymeric
material system due to nonbond interchain interactions.
To determine the cohesive energy densities for the two
beads, a series of molecular dynamics calculations are
carried out, one based on 20 Abead long molecular chains
and the other based on 50 Bbead long molecular chains.
The respective cohesive energy densities are obtained by
averaging the molecular dynamicsbased values calculated
over a time period of 1 ns. The resulting cohesive energy
density values (260.05 and 71.73 J/cm 3 ) for beads A and B,
respectively, were validated using Synthia computer program
from Accelrys [15] which employs the socalled
Quantitative Structure Activity and Property Relationships
(QSAR/QSPR) semiempirical method to calculate physicochemical
properties of polymers using the information
about their topology. The cohesive energy density results
obtained using Synthia were 285.05 and 68.73 J/cm 3 for
beads A and B, respectively. In all the subsequent calculations,
cohesive energy densities were set equal to the
values obtained by averaging the molecular dynamicsbased
and Synthiabased values. The procedure employed
in this section yielded an average value of the Abead/
Bbead unitless Flory–Huggins interaction parameter of
5.42. The corresponding meanfield energetic interaction
between beads is then calculated by multiplying this value
of the Flory–Huggins parameter with the product of the
universal gas constant and absolute temperature and by
dividing the result by V ref.
Problem formulation
J Mater Sci
Since the primary output of mesoscale modeling is the
prediction of nanometertomicronscale phase separation
phenomena, it is used in the present work to study the
formation of hard domains (and the soft matrix) from the
initially homogeneous state of polyurea. As mentioned
earlier, physical and mechanical properties of polyurea are
highly sensitive to the details of its microstructure while
the microstructural details are also highly sensitive to the
polyurea chemistry. Hence, the use of the mesoscale
computational method offers an opportunity for elucidating
relationships between the material chemistry and its
microstructure (and, to a lesser extent, relationships
between materials microstructure and its properties). An
example of a typical phaseseparated mesoscale microstructure
obtained in the present work is displayed in
Fig. 7a.
J Mater Sci
(a)
(b)
Fig. 7 a A nanometertomicron scale twophase microstructure
obtained using the mesoscale computational analysis; and b the
corresponding finite element model
Continuum scale calculations
As mentioned above, the primary results of mesoscale
analysis pertain to the prediction of the material nanometertomicron
scale microstructure. To establish quantitative
relations between such microstructure and the material
(effective) properties, continuumlevel approaches are used
in conjunction with the material constitutive relations for
the two constituent phases (as derived via the use of
atomicscale calculations). There are several wellestablished
continuumlevel methods for computation of the
effective material properties (e.g., [16, 17]). In the present
work, a modified version of the method described in Ref.
[16] is utilized.
Computational cell
The first step in the present continuumlevel computational
procedure involves mapping of the mesoscale material
microstructure onto a finite element mesh. The finite element
mesh used in the present work consists of eightnode
cubic elements (‘‘voxels’’). The edge length of the voxels is
chosen to be a relatively small fraction of the bead length.
During mapping of the discrete beadbased mesoscale
microstructure into the corresponding continuum finite
element model, each voxel is filled with material associated
with a bead whose centerpoint is closest to the centerpoint
of the voxel in question. To reduce stress concentrations
associated with the step/terrace character of the
harddomain/softmatrix interface, a procedure is devised
to smoothout these interfaces by controlled distortions of
the voxels. An example of the typical phasesegregated
continuumlevel microstructure obtained in the present
work is displayed in Fig. 7b. A close similarity between the
mesoscale computational cell displayed in Fig. 7a and the
corresponding finiteelement computational cell shown in
Fig. 7b is apparent.
The continuumscale computational method
To determine the effective properties of the microphasesegregated
polyurea, the computational cell displayed in
Fig. 7b is subjected to a number of quasistatic deformation
modes (while imposing periodic boundary conditions
across the cell faces) and the corresponding stress versus
strain curves are generated. More details regarding the
deformation modes used will be presented in ‘‘Results and
discussion’’ section, while additional details regarding the
finite element method employed can be found in Ref. [16].
All calculations carried out in this portion of the work
employed ABAQUS/Standard, a commercial (static) finite
element package [18].
Continuumlevel constitutive relations for the two
constituent phases
As will be shown in ‘‘Continuumlevel calculations’’ section,
the material constitutive models for the soft matrix
and the harddomain materials were found to be available
within the ABAQUS/Standard material library and, hence,
the atomicscale results only provide the needed parameterization
of these models.
Problem formulation
As mentioned above, the main task at the continuumlevel
was to carry out finiteelement analysis of few basic
123
deformation modes to determine effective properties of
polyurea associated with its microstructure obtained
through the use of mesoscale computational analysis.
Results and discussion
Atomicscale calculations
As mentioned earlier, the two main objectives of using
atomicscale calculations were: (a) determination of the
mesoscale morphological and interaction parameters; and
(b) determination and parameterization of the material
models for the soft matrix and the hard domains, the two
main phases in bulk polyurea. Utilization of the atomicscale
calculations in conjunction with the objective (a) was
discussed in ‘‘Mesoscale calculations’’ section, while their
use in objective (b) will be discussed here.
To determine the mechanical properties of the two
phases, the atomicscale computational cell was subjected
to a variety of deformation modes (e.g., uniaxialstrain
tension/compression, planestrain tension/compression,
simple shear, etc.) over a relatively large range of strains.
An example of the typical results pertaining to the
molecularlevel microstructure, in the soft matrix and the
hard domains after axial tension and simple shear are
shown in Fig. 8a–d.
Fig. 8 Relaxed atomic
configurations of the soft matrix
(a, b) and the hard domains
(c, d)within the computational
cell after: a, c axial tension;
and b, d simple shear
123
(a)
(c)
Softmatrix material model
The soft matrix was found to be capable of undergoing
large elastic strains and, hence, was treated as a hyperelastic
material. Strains are deemed as being elastic if
deformation of the computational cell followed by its full
restoration to the initial state does not result in any changes
of the atomic nearest neighbors. Following standard practice
[19], the volumetric internal strain energy density
(strainenergy density, in the following) of this phase is
assumed to be a function of the invariants (I1, I2, I3) of the
left Cauchy deformation tensor, B (= FF T ) where F is the
deformation gradient and superscript T denotes a transpose.
The deformation gradient F simply maps the initial undeformed
computational cell into the corresponding
deformed computational cell. The three B invariants are
defined as:
I1 ¼ trðBÞ ð2Þ
I2 ¼ 1
2 I2 1 trðB 2 Þ ð3Þ
I3 ¼ detðBÞ ð4Þ
where tr and det are used, respectively, to denote trace and
determinant operators.
The computed internalenergy density, W, data are used
to derive a W(I1,I2) function while recognizing that in the
Soft Matrix Axial Tension Soft Matrix Simple Shear
Hard Domain Axial Tension
(b)
(d)
Hard Domain Simple Shear
J Mater Sci
J Mater Sci
Left Cauchy Deformation Tensor Invariant, I 2
10
9
8
7
6
5
10
4
30
1010
1010
30
nearly incompressible polyurea, I3 * 1.0. The function
was found to be consistent with the following truncated
quadratic function of I1 and I2:
WðI1; I2Þ ¼c1ðI13Þþc2ðI23Þþc3ðI13ÞðI23Þ ð5Þ
with c 1 = 15.4 ± 1.1 MPa, c 2 =8.44 ± 0.7 MPa, and
c3 = 0.82 ± 0.05 MPa where the number following the
±symbol denotes one standard deviation of the quantity in
question. A contour plot showing the obtained W(I 1,I 2)
relationship is displayed in Fig. 9. Once W(I1,I2) function is
defined, the corresponding Cauchy stress versus largedeformation
(logarithmic) strain relation can be obtained
by proper differentiation of Eq. 5 and through the use of
chain rule [20].
Harddomains material model
3030
5050
7070 70
3
3 4 5 6 7 8 9 10
Left Cauchy Deformation Tensor Invariant, I1 Fig. 9 A functional relationship between the strain energy density
(MPa) and the first two invariants of the left Cauchy deformation
tensor in the soft matrix of polyurea
In the case of hard domains, it was found that, at relatively
small strains, inelastic deformations begin to dominate the
mechanical response of this material. Hence, this phase is
modeled as an isotropic elastic–plastic material and the
internalenergy density taken to be a quadratic function of
the strain components (with zero constant and linear
terms). For an isotropic linear elastic material, the quadratic
coefficient (a fourthorder elasticstiffness tensor)
contains only two independent parameters (selected here as
the Young’s modulus, E and the Poisson’s ratio, m). These
two parameters were obtained by subjecting the computational
cell to a set of uniaxial stress deformations and by
fitting the computed W value to the quadratic function
90
90
mentioned above. This procedure yielded the following
values: E = 48 ± 2.5 MPa and m = 0.38 ± 0.03. To validate
these results, W values were also computed for the
case of the computational cell subjected to simple shear.
The resulting shear modulus, G, was found to be fully
consistent with its expected value (=E/2(1 ? m)).
As far as the flowstrength of harddomains is concerned,
no significant strainhardening effects were
observed and both uniaxial stress and simple shear deformation
models yielded consistent yield strength values of
16.1 ± 2.3 MPa. It is generally believed that, at sufficiently
large stresses/strains, real polyurea undergoes
plastic deformation [20] and that this type of deformation is
localized within hard domains. While, the hard domain
yield strength is typically determined indirectly by fitting
the experimental data for polyurea, this quantity is determined
directly in the present work by carrying out atomicscale
computational mechanical tests on the harddomain
material.
Mesoscale calculations
As mentioned earlier, the main output of the mesoscale
calculations is the nanometerto micron scale material
microstructure. Typical mesoscale computational results
displayed in Fig. 7a reveal that the initially fully mixed
homogeneous material has microphasesegregated into
discrete ‘‘peanutshaped’’ hard domains distributed within
a continuous matrix. An example of the hard domain
morphology is presented as an inset in Fig. 7. This morphology
is fairly consistent with the one observed experimentally
in our ongoing research [21]. In addition, the
characteristic size (5–20 nm in length, 3–5 nm lateral
dimension) of the ‘‘peanutshaped’’ hard domains observed
in Fig. 7a is consistent with their experimental counterpart.
Continuumlevel calculations
It is well established that the effective mechanical response
of heterogeneous materials such as microphase segregated
polyurea is dependent on the properties of the constituent
materials and the material microstructure. In ‘‘Atomicscale
calculations’’ section, atomicscale computational
results were used to construct material models for the two
bulkpolyurea constituents, i.e., the soft matrix and the hard
domains. In ‘‘Mesoscale calculations’’ section, mesoscale
computations were employed to generate microphase
segregated microstructure of the polyurea. In this section,
finiteelement calculations are employed to determine the
effective quasistatic mechanical properties of bulk polyurea
and to compare the results with their experimental
counterparts in order to provide a proof of concept. In these
calculations, in accordance with the findings presented in
123
‘‘Atomicscale calculations’’ and ‘‘Mesoscale calculations’’
sections, the soft matrix is modeled as a polynomialtype
hyperelastic material while the hard domains are
treated as an isotropic linearelastic/idealplastic material.
Since these models are already available in ABAQUS/
Standard, only their parameterization, as determined in
‘‘Atomicscale calculations’’ and ‘‘Mesoscale calculations’’
sections had to be provided.
However, before this task can be accomplished, the
procedure outlined in ‘‘Computational cell’’ section had to
be employed to construct the appropriate twophase finite
element model. An example of the finite element model
obtained using this procedure is displayed in Fig. 7b. By
subjecting the computational cell displayed in this figure to
a variety of deformation modes and by measuring its
mechanical resistance to deformation (via the use of quasistatic
finiteelement analysis), one can gain a detailed
insight into the (quasistatic) mechanical response of the
microphasesegregated polyurea. In other words, the finite
element analysis can be employed to carry out a variety of
computational mechanical tests on the twophase polyurea.
To establish the validity of this approach, one must demonstrate
that the results of these computational mechanical
tests are consistent with their experimental counterparts.
Such validation was carried out in the present work and its
details are presented in the remainder of this section.
To validate the present computational mechanicaltesting
procedure, the (10 3 s 1 strainrate) uniaxial compression
loading/unloading tests carried out by Yi and
Boyce [22] are simulated using the computational cell
displayed in Fig. 7b and by performing the finite element
computations. A comparison between the computational
and the experimental results is shown in Fig. 10. It is seen
that the computed loading/unloading stress–strain response
displays similar behavior as that found experimentally by
Yi and Boyce [22]. Specifically, in both the computed and
the experimental results loading is initially associated with
a stiff response of the material. At larger strains, both the
computed and the experimental results show a gradual loss
of stiffness due to interplay between the geometrical and
material nonlinear effects. A similar level of agreement is
observed in the unloading behavior of polyurea. Namely,
the rate of unloading is initially quite high and subsequently
decreases as unloading proceeds. The quantitative
agreement between the two sets of results, however, can be
described as only fair. Overall, these findings are encouraging
since no polyureabased experimental data/parameters
were used in the present computational approach.
Future work
The procedure described above enables determination of
the mechanical response of the twophase polyurea unit
123
Cauchy Stress, MPa
10
8
6
4
2
Experimental [21]
Computational [Presentwork]
0
0 0.25 0.5 0.75 1
Log arithmic Strain, No units
Fig. 10 A comparison between the quasistatic uniaxial compression
stress versus strain results obtained experimentally in Ref. [22] and
computationally in the present work
cell subjected to any given state of deformation. Unfortunately,
in most reallife computer aided engineering analyses
such as interactions between an airborne blast wave
and a soldier’s (helmetprotected or unprotected) head,
impact of a projectile on to a polyureacoated military
vehicle body, etc., one cannot afford to use finely meshed
unit cellbased finiteelement models. Instead, a homogenized/smearedout
response of the twophase polyurea is
needed so that the number of elements in the finiteelement
mesh is manageable. Derivation of such a homogenizedmaterial
constitutive model is beyond the scope of the
present work. Nevertheless, it should be noted that the
results obtained in the present work can be used in two
ways during derivation of such models: (a) atomicscalederived
mechanical properties of the two phases and the
mesoscalederived material microstructure could be used
as inputs to either a selfconsistent, e.g., [23] or a socalled
‘‘generalized method of cells’’ (e.g. [24]) homogenization
procedure; and (b) continuumlevel finiteelement results
can be treated as ‘‘experimental’’ results and used in a more
conventional ‘‘curvefitting’’ procedure. Both of these
approaches are being currently investigated in our ongoing
research and the results of this work will be reported in a
future communication.
Summary and conclusions
J Mater Sci
Based on the results obtained in the present work, the
following summary remarks and main conclusions can be
drawn:
J Mater Sci
1. A threestep computational procedure combining
atomicscale, mesoscale, and continuumlevel analyses
of the material mechanical response and microstructure
evolution is introduced and used to determine
effective material properties of the microphase
segregated polyurea.
2. At the atomicscale, computational material tests are
carried out to determine the mechanical response of
the two polyurea phases, a soft matrix and the hard
domains.
3. At the mesoscale, the process (and the product) of
decomposition of an initially fully mixed polyurea into
its twophase segregated microstructure is carried out.
4. At the continuumlevel, quasistatic finite element
analyses are employed to determine the effective
mechanical properties of the twophase polyurea. The
use of these results in constructing a homogenized
(smearedout) continuumlevel material model for
microphase separated polyurea is also discussed.
Acknowledgements The material presented in this paper is based
on work supported by the Office of Naval Research (ONR) research
contract entitled ‘‘Elastomeric PolymerByDesign to Protect the
Warfighter Against Traumatic Brain Injury by Diverting the Blast
Induced Shock Waves from the Head’’, Contract Number 4036CU
ONR1125 as funded through the Pennsylvania State University, the
Army Research Office (ARO) research contract entitled ‘‘Multilength
Scale Material Model Development for Armorgrade Composites’’,
Contract Number W911NF0910513, and the Army
Research Laboratory (ARL) research contract entitled ‘‘Computational
Analysis and Modeling of Various Phenomena Accompanying
Detonation Explosives ShallowBuried in Soil’’ Contract Number
W911NF0620042. The authors are indebted to Drs. Roshdy
Barsoum of ONR and Bruce LaMattina of ARO for their continuing
support and interest in the present work. The authors also want
to thank professors J. Runt, J. Tarter, G. Settles, G. Dillon, and
M. Hargether for stimulating discussions and friendship.
References
1. Ryan AJ (1989) Polymer 31:707
2. Grujicic M, Bell WC, Pandurangan B, He T (2010) J Mater Des.
doi:10.1016/j.matdes.2010.05.002
3. Grujicic M, Pandurangan B, He T, Cheeseman BA, Yen CF,
Randow CL (2010) Mater Sci Eng A 527:7741
4. Roland CM, Cassini R (2007) Polymer 48:5747
5. Sun H (1998) J Phys Chem B 102:7338
6. Sun H, Ren P, Fried JR (1998) Comput Theoret Polym Sci
8(1/2):229
7. Materials Studio (2009) Visualizer Manual. Accelrys Inc.,
Princeton, NJ
8. Materials Studio (2009) Amorphous cell theory manual. Accelrys
Inc., Princeton, NJ
9. Grujicic M, Sun YP, Koudela KL (2007) Appl Surf Sci 253:3009
10. Materials Studio (2009) Discover theory manual. Accelrys Inc.,
Princeton, NJ
11. Theodorou DN, Suter UW (1986) Macromolecules 19:139
12. Malcolm GN, Rowlinson JS (1957) Trans Faraday Soc 53:921
13. Materials Studio (2009) Mesodyn theory manual. Accelrys Inc.,
Princeton, NJ
14. Hildebrand JH (1919) J Am Chem Soc 41:1067
15. Materials Studio (2009) Synthia manual. Accelrys Inc., Princeton,
NJ
16. Grujicic M, Zhang Y (1998) Mater Sci Eng A 251:64
17. Grujicic M, Cao G, Fadel GM (2002) J Mater Des Appl 215:225
18. ABAQUS/Standard Version 6.81 (2008) User Documentation,
Dassault Systems
19. Grujicic M, Bell WC, Pandurangan B, Glomski PS (2010)
J Mater Eng. doi:10.1007/s116650109724z
20. Grujicic M, Pandurangan B, He T, Hunt J, Tarter J, Dillon G
(2010) J Mat Des Appl (submitted)
21. Runt J (2010) Research in progress, Pennsylvania State
University
22. Yi J, Boyce MC, Lee GF, Balizer E (2006) Polymer 47:319
23. Bensoussan A, Lions JL, Panicolaou G (1978) Asymptotic
analysis for periodic structures. North Holland, Amsterdam
24. Wilt TE, Arnold SM (1996) Micromechanics Analysis Code
(MAC) User Guide: version 2.0., NASA TM107290
123